Effects of Palm Kernel Shell on the Microstructure and
Mechanical Properties of Recycled Polyethylene/Palm
Kernel Shell Particulate Composites
Agunsoye J. Olumuyiwa*, Talabi S. Isaac, Obe A. Adewunmi, Adamson I. Ololade
Department of Metallurgical and Materials Engineering, University of Lagos, Lagos, Nigeria Email: *firstname.lastname@example.org
Received May 16, 2012; revised June 30, 2012; accepted July 20, 2012
The effect of palm kernel shell on the microstructure and mechanical properties of recycled polyethylene (RLDPE) re-inforced with palm kernel shell particulate composite was evaluated to assess the possibility of using it as a new mate-rial for engineering applications. The composites were produced by compounding and compressive moulding technique by varying the Palm kernel shell particle from 5 - 25 vol% with particles size of 150, 300 and 400 µm. The microstruc-ture (SEM/EDS) and the mechanical properties of the composites were investigated. The hardness of the composite increases with increase in palm kernel shell content and the tensile strength of the composite increased to optimum of 5 vol%. Scanning electron Microscopy (SEM) of the composites surfaces indicates fairly interfacial interaction between the palm kernel shell particles and the RLDPE matrix. The composites produced with 150 µm particle size have the best properties of the entire grade. Hence this grade can be use for interior applications such as car seat, dash board, and car interior for decorative purposes or other interior parts of automobile where high strength is not considered a critical re-quirement.
Keywords: Recycled Polyethylene; Palm Kernel Shell; Microstructure and Properties
Composites are materials that comprise strong load car-rying material (known as reinforcement) imbedded in weaker material (known as matrix). Reinforcement pro-vides strength and rigidity, helping to support structural load. In recent years, due to growing environmental aware-ness, agro-fillers (agro-based waste) have been increas-ingly used as reinforcing fillers in thermoplastic compos-ite materials [1-2].
Natural fibers, as reinforcement, have recently attracted the attention of researchers because of their advantages over other established materials. They are environmen-tally friendly, fully biodegradable, abundantly available, renewable and cheap and have low density. Natural fiber composites are used in place of glass mostly in non- structural applications. A number of automotive compo-nents previously made with glass fiber composites are now being manufactured using environmentally friendly composites . This may be attributed to low-weight ratio of the composites.
Thousands of tons of different crops are produced but most of their wastes do not have any useful utilization.
Agricultural wastes include wheat husk, rice husk, and their straw, hemp fiber and shells of various dry fruits Mechanical properties of plant fibers are much lower when compared to those of the most widely used com-peting reinforcing glass fibers. However, because of their low density, the specific properties (property-to-density ratio), strength, and stiffness of plant fibers are compara-ble to the values of glass fibers [3-4]. Plant fibers are light compared to glass, carbon and aramid fibers. The biode-gradability of plant fibers can contribute to a healthy ecosystem while their low cost and high performance fulfill the economic interest of industry.
tuting a serious threat to environmental health of the na-tion. The purpose of the research is to explore the poten-tial of using palm kernel shell (powder) as reinforcement in polymer matrix composite for the development of new engineering material for the car interior.
2. Experimental Procedure
The palm kernel shell was dried and grinded into powder using a pulverizing machine, the powder was sieved in accordance with BS1377:1990 standard [7-8]. The recy-cled polyethylene was sun-dried and shredded in a plastic crusher machine. The palm kernel shell powder and the grinded pelletized recycled polyethylene were blend to-gether using a two-roll rheomixer at 165˚C and a rotor speed of 60 rpm. The percentage of the kernel shell par-ticles in the matrix was varied from 5% - 25% and five samples each were compacted using 150 µm, 300 µm, 400 µm. Compression of the composites was carried out in a Wabash V200 hot press for 5 minutes under con-trolled pressure 30 tons at 175˚C. Each of the samples was cooled to room temperature under pressure before it
an interval of 24 hrs for 168 hrs. The water absorption rate was then determined using Equation (1) .
final weight initial weight
%weight gained 100
3. Result and Discussion
The morphology of the developed composites are shown in Plates 1-7. From the morphology it, can be seen from the Scanning Electron Microscope results that homoge-neity between the kernel shell particles and the matrix decreases with increase in the kernel shell particles con-tent. The mwicrostructure clearly shows that when the kernel shells particle was added to the recycled polyeth-ylene (RLDPE) morphological change in the structure take place. The microstructure of the RLDPE matrix re-veals chain of lamellae and interlammeller amorphous structure with linear boundaries between adjacent spher-ulites boundaries (see Plate 1). From the EDS spectrum it can be clearly see that the functional group of the RLDPE were revealed.
Plate 1. EDS/SEM morphology of the recycled polyethylene.
Plate 2. EDS/SEM morphology of the recycled polyethylene reinforced with 10 vol% at 150 µm size.
Plate 3. EDS/SEM morphology of the recycled polyethylene reinforced with 25 vol%, 150 µm size.
Plate 5. EDS/SEM morphology of the recycled polyethylene reinforced with 20 vol%, 300 µm size.
Plate 6. EDS/SEM morphology of the recycled polyethylene reinforced with 15 vol%, 400 µm size.
Plate 7. EDS/SEM morphology of the recycled polyethylene reinforced with 25 vol%, 400 µm size.
The microstructure reveals that there are small discon-tinuities and a reasonably uniform distribution of parti-cles and the RLDPE. The partiparti-cles phase is shown as white phase, while the resin phase is dark. The kernel shell particles are embedded within the amorphous ma-trix composed of randomly distributed in the mama-trix pla-nar boundaries. The surface of the agro-waste particles is fairly smooth indicating that the compatibility between particles and the RLDPE was not so good. It can be seen that the agro-waste particles are not detached from the RLDPE surface as the volume fraction of kernel shell particles increased in the RLDPE, from the microstruc-ture it was observed the smallest particles size has good interfacial bonding them the biggest particle size.
The particle size of the reinforced (palm kernel shell particles) has significant effect on the strength, hardness, and impact energy of the composite. From Figure 1, it can be seen that the tensile strength of the composite increases
upto a maximum of 5 vol% of palm kernel shell particles within the matrix of the recycled polyethylene. The ten-sile strength of composites with 150 µm size palm kernel shell particles showed higher value, this is because of increasing in the surface area. This may also account for the good distribution and dispersion of the palm kernel shell particles in the RLDPE matrix resulting in strong- particles-RLDPE matrix interaction. This good particles dispersion will improve the particles-RLDPE matrix in-teraction and consequently increases the ability of the particles to restrain gross deformation of the RLDPE matrix. Nevertheless the tensile strength obtain in this study remained within acceptable levels for car interiors [8-10].
As expected, the yield strength varies directly with the tensile strength of the samples (See Figure 2). The yield strength slightly decreased as the vol% of palm kernel shell particles increased in the RLDPE matrix.
Figure 1. Effect of filler addition on the tensile strength of particulate palm kernel reinforced polyethylene composite.
tent within the matrix of the recycled polyethylene com-posite. The sample with 25 vol% at 400 µm particle size has the lowest impact energy. High strain rates or impact loads may be expected in many engineering applications of polymer composite materials. The suitability of a polymer composite for such applications should therefore be determined not only by usual design parameters, but by its impact or energy absorbing. These results are in agreement with the work of other researchers [8-10].
The rate of water absorption of the composite over a period of 168 hours at an interval of 24 hours increased with increased in kernel shell particles content in the composite. This may be due to imperfect interfacial bonding between the palm kernel shell particle and recy-cled polyethylene matrix. Also the water absorption is due to the hydrophilic nature of the palm kernel shell (See Figure 5). The swelling that occurs during the water absorption is the sum of two components, namely, swell-ing by hygroscopic particles and the release of compres-sion stresses imparted to the composites during the pressing of mat in the hot press. The release of compres-sion stresses, known as spring back, is not recovered when the composites is in a dry state.
Figure 3. Effect of filler addition on the hardness of par-ticulate palm kernel reinforced polyethylene composite.
Figure 4. Effect of filler addition on the impact strength of particulate palm kernel reinforced polyethylene composite.
Figure 5. Effect of filler addition on the rate of absorption of particulate palm kernel reinforced polyethylene compos-ite.
From the result of the investigations and discussion, the following conclusion has been made.
1) This work successfully shows that the fabrication of RLDPE and the palm kernel shell particles composite by compounding and compression moulding is feasible.
2) The uniform distribution of palm kernel shell particle in the microstructure of the composite is the major factor responsible for the increase in strength.
3) Palm kernel shell improves the hardness property of the recycled polyethylene matrix composite.
4) The tensile strength increased up to an optimum of 5 vol% and the composite produced with 150 µm particle size has the best properties of the entire grade. Hence this grade can be use for interior applications such as car seat, dash board, and car interior for decorative purposes or other interior parts of automobile where high strength is not considered a critical requirement.
 U. Johnson, H. Mahmud and Z. Mohd, “Enhancement and Prediction of Modulus of Elasticity of Palm Kernel Shell Concrete,” Materials and Design Journal, Vol. 32, No. 4, 2010, pp. 2143-2148.
 H. Larbig, H. Scherzer, B. Dahlke and R. Poltrock, “Natu-ral Fiber Reinforced Foams Based on Renewable Re-sources for Automotive Interior Applications,” Journal of Cellular Plastics, Vol. 34, No. 4, 1998, pp. 361-379.
 D. Rozman, A. Zainal and S. Umaru, “Natural Fibers, Biopolymers, and Biocomposites: Oil Palm Fiber-Thermo- plastics Composites,” CRC Press, Boca Raton, 2005.
 P. Wambua, U. Ivens and I. Verpoest, “Natural Fibers: Can They Replace Glass in Fiber-Reinforced Plastics?” Composites Science and Technology, Vol. 63, No. 9, 2003, pp. 1259-1264.
 P. Wambua, B. Vangrimde, S. Lomov and I. Verpoest, “The Response of Natural Fiber Composites to Ballistic Impact by Fragment Simulating Projectiles,” Composite Structures, Vol. 77, No. 2, 2007, pp. 232-240.
 R. Kozlowski and M. Helwig, “Lignocellulosic Polymer Composite,” In: P. N. Prasad, Ed., Science and Technol-ogy of Polymers and Advanced Materials, Plenum Press, New York, 1998, pp. 679-698.
 M. M. Davoodi, “Conceptual Design of a Polymer Com-posite Automotive Bumper Energy Absorber,” Materials & Design, Vol. 29, No. 7, 2008, pp. 1447-1452.
 D. J. Andrea and W. R. Brown, “Material Selection Proc-esses in Automotive Industry,” Michigan Transportation Research Institute, Ann Arbor, 1993.
 E. W. Godwin and F. L. Matthews, “Review of the Strength of Joints in Fibre-Reinforced Plastics: Part 1 Mechanically Fastened Joints,” Composites, Vol. 11, No. 3, 1980, pp. 155-160.doi:10.1016/0010-4361(80)90008-7